**Moisture Transport in Wood **

**and Wood-based Panels **

**A Mathematical Model of Hygroscopic **

**A Mathematical Model of Hygroscopic**

**Moisture Transport in Conifer Wood **

**Moisture Transport in Conifer Wood**

**BYGGNADSMATERIALLÄRA **

**K U N G L I G A T E K N I S K A H Ö G S K O L A N**

**1 0 0 4 4 S T O C K H O L M**

**TRITA-BYMA 1988:5**

## Trätek

**I N S T I T U T E T F Ö R T K A I 1 K N I S K 1 ( ) R S K N I N (**

**MOISTURE TRANSPORT IN WOOD AND WOOD BASED PANELS **
**- A mathematical model of hygroscopic moisture transport **
**in conifer wood **

**TräteknikCentrum, Rapport I 8810063 **

**Kungl Tekniska Högskolan, Rapport TRITA-BYMA 1988:5 **

**Keywords **

*diffusion *

*Itonber *

*mathematioal models *

*moisture movement *

*softuoods *

**Stockholm October 1988**

**översikter, utvecklingar och studier. Publicerade **
**rapporter betecknas med I eller P och numreras **
**tillsammans med alla utgåvor från **
**Träteknik-Centrum i löpande följd. **

**Rapporter kan som regel beställas kostnadsfritt i **
**ett exemplar av medlemsföretag. Ytterligare **
**be-ställda exemplar faktureras. **

**Citat tillätes om källan anges. **

**Reports issued by the Swedish Institute for Wood ****Technology Research comprise complete accounts ****for research results, or summaries, surveys and ****stu-dies. Published reports bear the designation I or P ****and are numbered in consecutive order together with ****all the other publications from the Institute. **

**Member companies may generally order one copy ****of any report free of charge. A charge will be made ****for any further copies ordered. **

**Extracts from the text may be reproduced provided ****the source is acknowledged. **

**möbel- och övrig träbearbetande industri), **
**träfi-berskivor, spånskivor och plywood. Ett avtal om **
**forskning och utveckling mellan industrin och **
**Styrelsen för Teknisk Utveckling (STU) utgör **
**grunden för verksamheten som utförs med egna, **
**samverkande och externa resurser. **
**Träteknik-Centrum har forskningsenheter, förutom i **
**Stock-holm, även i Jönköping och Skellefteå. **

**The Swedish Institute for Wood Technology ****Re-search serves the five branches of the industry: ****saw-mills, manufacturing (joinery, wooden houses, ****fur-niture and other woodworking plants), fibre board, ****particle board and plywood. A research and **

**deve-lopment agreement between the industry and the ****Swedish National Board for Technical Development ****(STU) forms the basis for the Institute's activities. ****The Institute utilises its own resources as well as ****those of its collaborators and other outside bodies. ****Apart from Stockholm, research units are also **

### SUMMARY 2

### Svensk sammanfattning 2

### Nomenclature 3

### 1 INTRODUCTION 6

### 2 MODEL STRUCTURE 7

### 2.1 Representative volume-averaged tracheid 7

### 2.2 Molecular diffusion in the lumen 10

### 2.3 Knudsen diffusion through the pit chamber 12

### 2.4 Bound water diffusion 14

### 2.5 Moisture in wood and in the air 16

### 2.6 Equation of moisture transport in the steady state 20

### 3 SOLUTION OF THE MODEL EQUATIONS AND SOME

### RESULTS 23

### 3.1 Solution of the equations 23

### 3.2 Choice of the data of cell structural dimensions 24

### 3.3 Some results of simulations for spruce 26

### 3.4 Comparison with Bertelsen's experiments 33

### 3.5 Comparison with Siau's model 34

### 4 ANALYSES OF MOISTURE TRANSFER TROUGH

### MOVING A N D STILL AIR LAYERS 38

### 4.1 Moisture transfer under forced convection 38

### 4.2 Moisture diffusion through still air 44

### 5 DISCUSSIONS AND CONCLUSIONS 51

### A model of steady-state moisture diffusion in conifer woods is presented in this

### paper. It is based on the results of previous scientific research on various forms

### of diffusion processes combined with the knowledge of the microscopic cellular

### structure of conifer woods. The sophistication and flexibility of the model

### structure enable it to predict the moisture diffusivity of various coniferous

### wood species in the hygroscopic range at different temperatures. When the data

### describing the cell dimensional structure of certain wood are determined

### properly and regulated , good predictions of the diffusivity will be produced.

### Some simulations of the moisture diffusion of Scandinavian spruce are made

### in the three principal directions at several temperatures. Comparison of the

### resultant diffusivities with the experimental results of Berteisen (1984) and the

### predicted diffusivities of Siau's model has shown good similarities.

### Finally , as an attachment to the model, the resistance to moisture transfer

### through the boundary layer of flow air into or out of a wood lumber is analysed

### with boundary theory, and the resistance of moisture diffusion through the air

### space inside a cup (vapometer) are analysed with the equation of binary gaseous

### diffusion. The results of these investigations are expected to be able to serve for

### a better understanding of these two generally neglected problems i n the

### measurement techniques of the cup and sorption methods.

### SVENSK SAMMANFATTNING

Rapporten presenterar en matematisk modell för fuktdiffusion i barrved. Den är baserad på tidigare arbeten om olika diffusionsprocesser i kombination med kunskap om den mikroskopiska cellstrukturen hos barrved. Modellens nivå och mångsidighet gör det möjligt att förutsäga fuktdiffusiviteten inom det hygroskopiska området för olika typer av barrved och vid olika temperaturer. Då det finns data som beskriver dimensionerna i vedens cellstruktur korrekt, kan modellen förutsäga fuktdiffusiviteten.

Fuktdiffusiviteten i skandivinaisk gran har simulerats i vedens tre huvudriktningar vid olika temperaturer och jämförts både med experimentalla data av Berteisen (1984) och med en annan modell av Siau (1984). Överensstämmelsen är god. I ett separat avsnitt har övergångsmotståndet i ett gränsskikt nära träytan analyserats teoretiskt. Även övergångsmotståndet genom luftskiktet inuti koppen, då den s.k koppmetoden används för mätning av fuktdiffusion, har analyserats teoretiskt. Resultaten ska förhoppningsvis underlätta förståelsen av fenomen i samband med övergångsmotstånd, som ofta förbises då kopp- och sorptions-metoden används experimentellt.

### A, B, D lengths of three sections of the representative

### tracheid in the diffusion direction, figure 1

### Db bound water diffusivity, based on moisture

### concentration in wood cell substance

### D(w), 6(p) moisture diffusivities in wood , based on

### mois-ture concentrations in gross wood and in the air

### D/f^ effective diffusivity of bound water in cell wall,

### in section A of the representative tracheid, figure 1

### Db^ff effective diffusivity of bound water, in section B

### D/ff effective diffusivity of bound water, in section D

### Eb activation energy of bound water

**FSP fiber saturation point **

### g moisture flux

### G specific gravity of wood

### Go specific gravity of ovendry wood

### m

### m^s

**mVs**### mVs

**mVs**### J/mol

%### kg/m^s

### height of the air space inside a cup, figure 15

_{m }

### L

### Mw

### n

### Na

### length of a lumber in the air flow direction

### molecular weight of water, equal to 0.01802

### porosity of solid wood

### mass flux of water vapor

### molar flux of the air

### molar flux of water vapor

### m

### kg/mol

### kg/m^s

### mol/m^s

### mol/m^s

**Pt total gas pressure **

**Pg saturation water vapor pressure in the air **

**T2 effective radius of aperture-pit chamber system **

**T2 effective radius of aperture-pit chamber system**

### r3 effective radius of margo pore

### R gas constant, equal to 8.31441

**S, Sj, S2 areas of various components of the **

**represen-S3, S4, S5 tative tracheid in diffusion direction, figure 1 **

### SJ a parameter defined in Eq( 14)

### S^, Sh fractional volumetric swelling and shrinkage

### of solid wood between zero moisture content

### and

**F S P**

**Pa**

**Pa**

### m

### m

### J/molK

### m^

### Tc temperature in Celsius C

### u moisture content in wood, based on dry wood %

### weight

### Uf moisture content at FSP %

### U air velocity m/s

### w moisture concentration in wood, based on wet kg/m^

### volume

**Wq, Wji moisture concentrations on the surfaces of the kg/m^ **

### model wood lumber, figure 5

### Xy molar fraction of water vapor in the air

### Y space coordinate m

### a attenuation factor, equal to the fraction of pits

### aspirated

### Pst mass transfer coefficient through still air m/s

### Pav average mass transfer coefficient through m/s

### boundary layer

### 5]^ Knudsen diffusivity m^/s

**5}^ Knudsen diffusivity of water vapor in the mVs **

**5}^ Knudsen diffusivity of water vapor in the mVs**

### aperture and pit chamber capillaric system

**Knudsen diffusivity through margo pores rnVs **

**Knudsen diffusivity through margo pores rnVs**

**8m molecular diffusivity of water vapor in the bulk air mVs **

**8m molecular diffusivity of water vapor in the bulk air mVs**

**5v diffusivity of water vapor mVs **

**5v diffusivity of water vapor mVs**

**b^^^i effective diffusivity of water vapor in lumen mVs **

**b^^^i effective diffusivity of water vapor in lumen mVs**

**b^^^2 effective diffusivity of water vapor in the aperture rnVs **

**b^^^2 effective diffusivity of water vapor in the aperture rnVs**

### and pit chamber capillaric system

**^^^^2 effective diffusivity of water vapor in margo mVs **

**^^^^2 effective diffusivity of water vapor in margo mVs**

### pores

**V kinematic viscosity of the air mVs **

**V kinematic viscosity of the air mVs**

### Pa molar density of the air under atmospheric mol/m^

### with moisture contents on the two surfaces of the

### modeled wood lumber, figure 5

### ps moisture concentration on the surface of a lumber, kg/m^

### figure 12

### poo moisture concentration in the bulk flow air, kg/m^

### figure 12

### pw normal density of water kg/m^

### XI tortuosity of lumen

**12 tortuosity of aperture-pit chamber capillaric system **

**X3 tortuosity of margo pores **

### <t) relative humidity of the air %

### <|) s relative humidity on the surface of a lumber, %

### figure 12

**(j) 00 relative humidity in the bulk flow air, figure 12 % **

### (t) t a parameter defined in Eq( 17)

### Note: Some sparsely used nomenclature is explained in the intimate context of

### the relevant equations and not listed here.

### Moisture transport in wood and wood composites assumes the form of diffusion under the

### fiber saturation point (FSP) which is entitled as the hygroscopic moisture range. In this

### moisture range, bound water diffuses in wood cell walls and water vapor diffuses in the

### lumen-margo pit capillaric system simultaneously. The cellular structure of wood is fairly

### regular: about 94 percent of the wood bulk comprises of longitudinal tracheids, with the rest

### being longitudinal canals and rays. These two facts can lead to a promising access to the

### mathematical modelling of hygroscopic moisture movement in the conifer woods.

### Solid wood is a kind of polymeric, bio-organic and porous material. The diffusion process of

### polymeric materials is in general regarded as an activated process that is frequently described

### with Arrhenius equation fitted with some experimentally or theoretically determined data of

### activated energy( in the case of diffusivity with exponential concentration dependency). The

### theories of moisture diffusion in the bulk air and gas diffusion through extremely tiny pores

### that exist in wood are both well developed. A combination of these theories with the

### knowledge of the cellular structure of conifer wood can produce a more precise

### comprehension of the moisture transport process in conifer woods.

### Simulation in this model is limited to isothermal diffusion in steady state along the three

### principal directions of conifer wood: tangential, radial, and longimdinal. This directly

### produces predicted moisture transport coefficient in the hygroscopic range: moisture

### diffusivities. Some examples of predicted diffusivities of average Scandinavian spruce in

### various climates are to be presented and compared with some available experimental data and

### with Siau's model.

### The resistance of moisture transport through stirred as well as still air, which exist in reality

### but are generally neglected in the measurement techniques of the cup and sorption methods,

### is to be analysed theoretically. They have nothing to do direcdy with the model. But since

### their contents are also in the study realm of moisture transport in woods, they are included in

### this paper as an attachment.

### In constructing the model, the stmctural features of conifer woods are to be considered. As

### woods are anisotropic, moisture diffusion along each of their three principal directions needs

### be accounted. The sizes of the capillaries inside wood are in three different magnitude orders,

### in which the diffusion mechanisms differ to some extent. Moreover, the hygroscopic water

### also moves inside the wood cell walls in a bound (adsorbed) state whenever there is a

### concentration difference. These diffusion forms are to be treated separatedly and then

### combined in the model based on a volume-average wood entity - the representative tracheid.

**2.1 Representative Volume-averaged Tracheid **

### The study of wood anatomy has revealed that longitudinal tracheids that are long, narrow

### and thick-walled wood cells make up nearly 94 percent of the bulk of conifer wood. We may

### consequently regard tracheids being the only components in conifer woods. This

### consideration can be modified by regulating some dimensional data of tracheid structure in

### account for the effect of 6 percent of the other cells.

### Consider a representative volume-averaged tracheid, whose dimension of cell wall, lumen

### and pit chamber are the average values of a certain wood species or a portion of this wood

### species, e.g., it can be heartwood or sapwood with or without aspiration, it can be wood

### from different parts of a stem etc. This definition plays a similar role to the representative

### elementary volume in the continuum approach for die theory of transport in porous media. It

### is possible to evaluate with reasonable certainty the data describing the dimensions of the

### representative volume-averaged tracheid, especially for Scandinavian spruce (Pice abies) and

### pine (Pinus silverstris) because Amber and Thömquist(1982), Boutelje (1983) and Bolton

### (1976) have made extensive investigations in this field. Siau (1984) and Cote (1965) also

### summarized and presented the dimensional data of conifer wood cells.

### Make a projection of this representative tracheid in the tangential and longitudinal directions

### (the radial projection is similar to the the tangential one, so it is omitted for simplicity),

### modify the projections by laying the areas of cell wall, pit chambers and membrane pores in

### each direction together as illustrated in figure 1. The modification is justified because it is

### equivalent to a tracheid structure if the connected cell wall of two adjacent cells are attributed

### to one tracheid and

### S4

f 1**y**

_{• }

**' y y**

**N \ >**

**' y y**

**\ \ >**

**• y y**

**X \ \**

### S3 Si s

**' y y**

**\ \ >**

**' y y**

**\ \ \**

**' y y**

**\ \ >**

**' y y**

**N N >**

**' y y**

**X X >**

**' y y**

**» y y**

**> y V ^**

**X N >**

**' y y**

**X \ >**

**y y**

**X X X**

_{y y y }X X X**X X •<**

**X \ X**

**' y y**

**X X X**

**• y y**

**X X X**

**y y y**

**X X X**

**y y y**

**N**

### •11< >

### DB A

### T

**Tangential **

**Projection **

**Logitudinal **

**Projection **

### Figure 1

### Dimensions of the representative volume-averaged tracheid and its modified projections

### in the tangential and longitudinal directions. The modification is in that the projected

### areas of the cell wall,pit chambers and pores in each direction are laid together. The

### arrows indicate the directions of moisture diffusion.

### S : area of the tracheid across diffusion direction

### S j : area of lumen across diffusion direction

**82: area of cell wall **

**S3: area of lumen minus the areas of pit chambers **

**84: sum of pit chamber areas minus pit areas **

**85: sum of margo pore areas **

### A : length of the lumen in the diffusion direction

### B : thickness of cell wall minus membrane thickness

### D : thickness of pit membrane

*tracheid A, B and D. Note that the aperture and the pit chamber are treated here as one *
stmctural component and projected together since the sizes of them are similar. The average
area of the aperture and the overall chamber is to be used for this component.

Most commercial woods have been subjected to kiln drying before use which makes a large
portion of pits aspirated. Pit aspiration reduces the area of margo pores available for vapor to
*go through. To consider this effect, an attenuation factor a is introduced which indicates the *
fraction of the pit aspirated. When a pit is aspirated we may regard it as having membrane
**without pores. The sum of chamber areas minus pore areas S4 and the sum of pore areas ****in figure 1 therefore need to be alterred in account for pit aspiration: **

**S*4 = 8 4 + Sjtt **

**5*5 = 85(1-a) **

Two other important parameters not indicated in figure 2 are the effective radii of the
**aperture-pit chamber rj and of the pore **

In the present model a block of solid conifer wood is assumed to be made up of a matrix of
**the representative tracheid in parallel and in series. 80 when diffusion in one representative **
tracheid is described along the three principal directions, the moisture transport in any
direction of the block will be determined.

**2.2 Molecular Diffusion in the Lumen **

**The diameter of tracheid is in the range of 8-35 [Lm. Water vapor move through the air inside **

**The diameter of tracheid is in the range of 8-35 [Lm. Water vapor move through the air inside**

### the lumen in the same way as it moves in the bulk air. The diffusivity of such molecular

### diffusion is:

### 5 = 2 . 2 0 x l O - ^ ( i ^ ) ( - I - ) ^ - ^ ^ (1)

_{^ V p V 275J5 ^ ^ }

### According to Pick's law, the unidirectional molar flux of vapor diffusion A^^ relative to

### stationary coordinate in a binary mixture like water vapor and air is (Bird, Steward and

### Lightfoot, 1960):

### dX

### N = X ( N + N ) - p 5 (2)

**V v"- V a'' ^a m**

**In wood the net flux of air is zero (8tanish, 1986), = 0. Thus die molar flux of vapor is: **

**In wood the net flux of air is zero (8tanish, 1986), = 0. Thus die molar flux of vapor is:**

### p 5 dX

### N = - l l i I L _ l (3)

### 1-X dY ^"^^

### V

### The mass flux of vapor expressed with mass concentration p is:

### n =

**-V**

### dp

### l-p/(p M J dY

### where is the molar density of the air that can be calculated with the ideal gas law, the

### molecular weight of water.

### In the representative tracheid ^ must be multiplied by the lumen area fraction and divided by

### a tortuosity in account for the area available for the molecular vapor diffusion and the

### probable non-straight path. The moisture flux in lumen is then simply expressed as:

**1**

### dY

### 1 - p/(p M

**J**

### S

**The term p/CpJ^J in Eq(3), (5) is not only proportional to moisture concentration p but **

**The term p/CpJ^J in Eq(3), (5) is not only proportional to moisture concentration p but**

### also rather strongly dependent on temperature. At a temperature below 50 °C, it is much less

### than unity and is probably negligible. But as temperature rises above 50 °C its value will be

### more and more near to unity, and is no longer excludable. For water vapor saturated air, the

**term p/iP(Mw) is equal to 0.0231,0.122 and 0.473 at 20 °C, 50 »C and 80 respectively. **

**term p/iP(Mw) is equal to 0.0231,0.122 and 0.473 at 20 °C, 50 »C and 80 respectively.**

**2.3 Knudsen Diffusion through Pit Chamber **

### For the tracheid the diameters of the border aperture, of tiie overall chamber and of the margo

### pores are in the ranges of 1.5-2.7 p.m, 8.0-17 p.m and 0.15-2.0 ^im respectively figure 2.

### These sizes are nearly in the same range as the mean free path of water vapor molecules at

### ordinary temperature at atmospheric pressure.

### 1

### k •

**Jr-k • **

**Figure 2 **

**Bordered pit on tracheid wall **

**Pit aperture **

**pit chamber **

**Pores on margo **

**torus **

### From molecular kinetic theory, it is known that vapor diffusion through die voids in the sizes

### of pit chambers and margo pores is opposed not only by the collision between gas molecules

### as in the case of molecular diffusion, but also by the collision of vapor molecules with the

### walls of die voids. The latter effect is described as the Knudsen diffusion (Hines and

### Maddox, 1985), die diffusivity of which is:

### 6^ = 9.70r(.

### lOOOM

### (6)

### The effective Knudsen diffusivity in the tracheid also equals to 5^ multiplied by void area

### fraction of the void and divided by a tortuosity. When the molecular diffusion and the

### Knudsen diffusion occur simultaneously, the molar vapor flux is (Satterfield, 1970):

**V **

### N = ^

### N dY

**AsN y= 0 in wood, the mass flux is: **

**AsN y= 0 in wood, the mass flux is:**

### n..=

** 1**

**1**

### ^ (7)

### l - p / ( p M J 1

**+**

**V k **

### Since the diameter of the membrane pores are one order smaller than that of the overall pit

### chamber (figure 2), it is treated as a separate structural component here while the aperture and

### the chamber together as a component. The reciprocal of the effective diffusivity in the

### aperture-pit chamber system is:

### 1 1-P/(PMJ 1 ,1-P/(P M J 1 _ S ^

**V**

**m k2 4 5**

### The reciprocal of the effective diffusivity in the margo pores is:

**1 1 - p/(p M ) 1 l-p/(p M ) 1 s **

**5 f ^ 3 85(1-a) ^ **

**Here 5^ and 5^ are equal to 5^ in Eq(6) when the diameter of the aperture-pit chamber r2 **

**and of the pore are substituted into it for respectively. The effect of the term pKPcMw) **

**and of the pore are substituted into it for respectively. The effect of the term pKPcMw)**

### Eq(8), (9) to rather small and much less pronounced than its influence to

**^ffi in Eq(5). This is because 6^^ is approximately two orders greater than ^^"^ **

**^ffi in Eq(5). This is because 6^^ is approximately two orders greater than ^^"^**

**2.4 Bound Water Diffusion **

The concentration of water inside cell walls in equilibrium with the ambient air is in the order

**of about 10,000 times larger than the water vapor concentration in the air. This makes the **

bound water diffusion important for wood in the overall hygroscopic moisture movement. Stamm(1959, 1960) systematically measured bound water diffusivity of eight wood species (among them four are conifer wood and the other four are hardwood) in the three principal directions at several temperatures. He found that the bound water diffusivity is identical for different wood species and that it changed with moisture content and temperature exponentially. Skaar and Siau (1981) fitted the data measured of Stamm into the Arrhenius equation and thus calculated the activation energy of bound water diffusion £^ as a function

**of moisture content u, which is shown in figure 3. **

**4 1 0 0 **
**3800 **
**QJ 3500 **
**o 3 2 0 0 **
**•5 2 9 0 0 h **
**2600 k **
**5 10 15 20 **
**M o i s t u r e C o n t e n t ( % ) **
**25 ** **30 **
Figure 3
The activation energy
of bound water diffusion

*Eh versus moisture *

content, calculated by fitting Stamm's data (1959) into the Arrhenius equation. The straight line is a linear approxi-mation.

(Skaar and Siau, 1981)

Skaar and Siau approximated the function with a linear relation Eb = 38519-293.1 u J/mol

To gain a higher accuracy, the curve in figure 3 is approximated by the present author with
sectional quadratic equations. Nine points are taken from the curve, among them special attenuation
*is paid to use the three points proposed by Stamm: £^ = 59775 J/mol at u =2 %, Ei, = 35588 at *

**4 2 1 0 7 - 1334.2U** +** 83.965u2** O < u < 6
E =** 4 0 1 9 7 - 5 8 9 . 0 1 U** +** 12.804u2** 6 < u < 1 6

**3 0 4 0 8** +** 556.32U - 20.542u2** 16 < u < 24

**- 6 0 1 2 2 + 7595.9U - 155.51u2 24 < u < **

With the above equation of activation energy, which would give reasonably accurate data in the
*range 2% < u< 28%, bound water diffusivity is expressed as: *

_ ^

D , = D , e (10)

Stamm found that the bound water diffusivity in longitudinal direction is approximately three
*times so large as that in tangential and two time as large as that in radial. At u= 20 % and T = *

**25.5 C, the longitudinal bound water diffusivity of conifer wood is 39 x lO-^^ irrespective of **

wood density and species. From Stamm's data in Eq(lO) is determined as:

**2 . 6 2 X 10-5 in longitudinal **

**Do = 8.73 X 10-6 in tangential ( 1 1 ) **

**1.31 X 10-5 in radial **

*Diy in Eq(lO) ought be multiplied by the cell wall area fraction in the bound water flux *

expression, but not divided by a tortuosity since the bound water diffusivity measured by
Stamm is believed to have incorporated the factor. Moreover, according to Siau** ( 1 9 8 4 ) ,** is
based on moisture concentration in wood cell substance. When used for moisture
*concen-tration in gross wood, it should be divided by a factor (1-n). Here n is the porosity of gross *
wood.

*The effective bound water diffusivity in the representative thacheid through section A, B, D *
**(parallel with the lumen, the pit chamber and the membrane pore respectively) in figure 1 are **
consequently:

**b S i _ n **

**82 + 83 + 8 4 + 8 5 0 1 **
**1 - n **

**2.5 Moisture in Wood and in the Air **

In this model the sorption equilibrium of moisture in the wood cell walls and in the air is rightfully assumed to be kept.

Many theories and models have been proposed to explain the sorption of water vapor for polymers and wood. One of them is Hailwood-Horrobin sorption theory, which suggests a sorption equation as:

W _ K , - l 1800 ^ K ,

C = - r !—=-1 i> 180000 + 1 '

* Here Kj^ K2 and W are constants at a certain temperature. Simpson(1971, 1981) fitted the *
sorption data of solid wood in the Wood Hand Book to the Hailwood-Hoirobin equation for a

*wide temperature range, and determined values of Kl, K2 and W as functions of the *
temperature in Celsius 7^:
K, = 4.738 + 0.04782T - 0.0004989T^
**1 c c **
**K . = 0.7094 + 0.002093T - 5.553 x 10" ^ **
**z c c **
W = 223.4 + 0.6942T +0.018531^
**c c **

* The Hailwood-Horrobin equation with the Ki K2 and W values correlated by Simpson has *
been proven to produce a good fit to sorption isotherm of solid woods between the temperature
of -2.8 °C and 147 °C. It is well accepted and utilized in North America. For example, in a
hand book with the title of Canadian Woods-Their Properties and Uses that is published by
University of Toronto Press (1981, third edition), a whole table of sorption isotherm data for
solid wood is made from this equation. A later edition of the Wood Hand Book:(1987) also
includes the equation.

This sorption equation is employed in this model to derive the analytical equilibrium relations of moisture concentration in wood w and in the air p.

According to Kollmann and Cote (1968), the volumetric swelling of pine and birch changes
linearly from zero moisture content to FSP, figure 4. Such linear swelling may be considered
as being true of average solid wood. When the fractional volumetric swelling of a wood
*species from zero moisture content to FSP is known, the volume of wood lumber V *
*with an oven dry volume at moisture content u is: *

S. V = V J 1 + — u )

0 u.

**w **

Here My is moisure content of wood at FSP that usually can be taken as 30% at room temperature. For Scandinavian spruce and pine Esping (1977) gave the value of 26 and 30% to

the sapwood and heartwood respectively. An average of 28% will be used in this model. The wood moisture content at FSP decreases approximately linearly 0.1 percent per degree rise in temperature. (Esping, 1977 and Siau, 1984). My of a wood with the value equal to M^^y at 20 °C can be expressed as:

Figure 4

Volumetric and linear swelling of pine and birch.

*Py'. Volumetric swelling of pine *
*By-. Volumetric swelling of birch *

Pt. Pr» P|" Tangential, radial and longitudinal swelling of pine. (Kollmann and Cote, 1968)

**^ *7**** ifO \ SO **

**Moisture content **

In several handbooks on wood drying, e.g.,. the one by Esping (1977), data of wood
fractional shrinkage 5;, from green wood to zero moisture content for many wood species
* are presented. Here we define a parameter ^j., which equals to the fractional volumetric *
swelling per percentage rise in moisture centent:

S S = ^ =

' (l-Sj^)Mf

Then the volume of lumber with respect to moisture content is:

(14)

*The specific gravity of a wood lumber G with dry specific gravity is: *
G V G

G ~

V (1 + S u) 1 + S u

**r ' r **

*The moisture concentration in wood w in relation to moisture content u is therefore: *

.^oPw, u

*T *

where p^^, is normal water density.

Employ the ideal gas law to water vapor, the relation of relative humidity 0 and moisture concentration in the air p is:

**For simplicity a parameter (f) [ is defined here that is constant at a constant temperature: **

lOORT

**s w **

is the saturation water vapor pressure, which can be obtained rather accurately with the Frost-Kalkwarf formula (Frost and Kalkwarf,1953):

**logPs = A -f- BA' -t- C X logT + D P / r 2 (18) **
A = 22.75017, C = -4.695517

Frost and Kalkwarf stated that their fomula could produce vapor pressures of various liquids from triple point (0 °C for water) to critical point (374. °C for water) with an average deviation of 0.3 percent from the experimental values. Check by the present author has shown that for water vapor this formula can give vapor pressure between O °C and -10 °C with maximum deviation less than 2 percent from the values in the Hand Book of Chemistry and Physics (1978).

The last term on the right hand side of the above formula is small compared with the rest, so is calculated with five cycles of succesive approximation in the computer. obtained with the formula has a unit of mm Hg. It is converted to Pascal only when the formula has been used in order to keep its accuracy.

*From Eq(13), (14), (15) and (16) the relation of w, p, dw/dp are deduced as: *

**w = Ä x (19) **

**100 A , + ( B , + S^np - C,(*,p)2 **

dw ^ [ N - ^ W ' ] dp ' ' [ A ^ + (B^ + Sp<t.,p-q(<t{p)']'

(20)

These two equations are used to correlate the moisture diffusion in the wood cell wall substance and in the air inside the capillaries of wood cells.

**2.6 Equations of Moisture Transport in Steady State **

^eff dw _eff dp . . »
g = - D ^ — - 5i — m section A
_eff dw eff dp r.
g = - D j , ^ - § 2 ^ m section B (21)
^eff dw _eff dp _
**g = -Dd dY • ^3 dY msecnon D **

The flux in Eq(21) need to be reexpressed with only one kind of concentration gradient,

*dp/dy or dw/dy. We define a function F(p) = dwidp from Eq(20), then: *

dw dw dp dp

**S - { D f x F ( p ) . 5 f , ^ = - 5 ^ ^ , ^ p ) ^ **

**g = - ( D f x F C p ) . 5 f ) | . = . 5 , , . „ ( p ) § in B (22) **

**g = - ( D r x F ( p ) . 6 f , ^ = . 5 , , , „ ( p ) ^ **

*A combination of the above flux expressions with the continuity equation dpidt = dgldy *
would give the diffusion equation of the present model. But in this paper we will not employ
this model to simulate moisture transport in any specific condition. Instead, we use it to some
general cases of steady-state moisture diffusion in conifer woods and then calculate the
moisture diffusivities from the obtained flux and moisture concentration data, which is
probably of more interest as the coefficients reveal the important property of the capacity of
woods in conducting moisture movement through them and may benefit the calculations of
moisture transport amount in the woods in practical uses.

We consider a piece of some conifer wood, on whose two surfaces moisture concentrations are maintained at constant values, as illustrated in figure 5. Moisture diffuses through the wood piece due to the concentration difference, and the diffusion has already lasted for such a sufficiently long time that steady state is reached.

**P **

### Sealing

### Figure 5

A piece of w o o d on whose t w o s u r f a c e s t h e m o i s t u r e c o n c e n t r a t i o n i s kept a t c o n s t a n t values.Since the moisture flux is constant in the steady-state moisture transport, we can equate the
*flux expression of each section (A, B, D) in any tracheid to tiiat of tiie next, and thus obtain a *
first-order, nonlinear differential equation group:

( \ e f f ( P ) - 8 h . e f f ( P ) } ^ = 0

**dp **

**(5b.eff(P)-5d,eff(P)}d7=0**( 8 d . e f f ( P ) - 8 . . e f f ( P ) } ^ = 0

**(S«ff(P)-5b,eff(P)}Z7=0**first tracheid (23) second tracheid

**( S a , e f f ( P ) - S h e . f f ( P ) } ^ = 0**

_{dY }last tracheid

**Boundary : P = Po at Y= 0**condition P = Pn at Y= L

This equation group is the expression of the present model for steady-state diffusion. The
*solution of it under given boundary conditions and at a certain temperature (T) will produce *
the moisture concentration distribution in the wood lumber. From this the effective diffusivity
of the model wood in the given concentration range and temperatiu'e can be derived.

**3. SOLUTION O F T H E M O D E L EQUATIONS **

**AND SOME R E S U L T S **

**3.1 Solution of th Equations **

To solve Eq(23), the numerical method for solving the nonlinear differential equation is
utilized. Eq(23) is firstly converted to a difference equation group. The space grid is directly
*taken asA,B,D that are the lengths of the three sections of the representative tracheid in *
diffusion direction. This approach is justified since the sizes of the tracheid are very small
compared to the wood lumber. The difference equations thus obtained are:

**^ a . e f f ( P , , , ^ ^ - T ~ - \ e f f ( P , , l ) - ^ - = 0 **
**W P , , i ) ^ - s . , f f ( P , ^ , ) - ^ = 0 **
**S c i . e f f ( P , , . ) ^ - 5 , , e f f ( P 3 , l ) ^ = 0 (24) **
Jv N** Pn-2 Pn-1** 5j

** V**

**Ri ^**

**\ e f f f r „ . 3 ) — B \ e f f ( P „ . ) — ^ = 0**p. + p. ,

### Where p , = l ^ f l i l

*-PQ and p„ are known, the number of equations and the unknowns are both (n-1). The *

nonlinear differential equation group has been converted into a nonlinear algebraic equation group. It is solved on computer with numerical method.

With the solution of Eq(24) the moisture concentration distribution** (po> Ph P2> ••> Pi> •••> **

p „ j in the wood lumber is derived. Thereafter the concentration dependent diffusivity is determined by means of numerical differentiation with relation:

**5(p) = Flux X — (25) **
dp

*The Flux is a constant that is obtainable in the process of solving Eq(24). *

The diffusivity calculated with Eq(25) is based on moisture concentration in the air, which is a requirement in the research of building materials. However in the wood drying research common interests are in the diffusivity based on moisture concentration in solid wood. Diffusivities expressed on the two bases can be easily converted from one to another with:

D(w) = 5(p)** X** ^ (26)

dw

*The analytical expression of dp/dw is Eq(20), with which D(w) is calculated directly from *

*S(p) in the simulation. As w is about 10,000 time larger than p, D(w) in general about *

*10,000 times less than S(p) in order of magnitude. *

**3.2 Choice of Data for Cell Structural Dimensions **

Amber and Thömquist (1982) made extensive measurements for tracheid lengths, widths and dry wood density of different parts of a spruce and a pine felled near Uppsala, Sweden. They found in the stems of the U-ee the following:

Spruce Pine Tracheid length 0.9 -3.9 mm 0.9 - 3.5 mm

Tracheid width 0.021 - 0.042 mm 0.023 - 0.042 mm Dry density 300 -590 kg/m^ 300 - 540 kg/m^

In the investigation of the effects of the membrane deformation and the sizes of pit chamber , pore and lumen on the permeability during fluids flow through conifer woods, Bolton (1976)

presented detailed data of the tracheid structural sizes for spruce (Pinus Silvestris), a part of them is directly from his own measurements. Siau (1984) also made summaries of tracheid structural dimensions. A portion of their data together with the data fed into the present model in simulating average Scandinavian spmce are listed in the table below.

Data of tracheid structural dimension from Bolton (1976), Siau (1984) and the

ones fed in the model (unit: (im)

Species Bolton(spruce) first formed earlywood center latewood

Siau This model conifer wood spmce DIAMETER: Aperture Overall chamber Torus Pore (effective) Lumen 2.70 17 8.5 0.30 30-35 1.5 8.0 4.0 0.40 8-25 6-30 0.01-4 20-30 2.5 14 6.0 0.2 27 Thickness of 0.21 membrane Number of bordered 100 pit per tracheid

Number of margo 200 per pit Tracheid length 4000 0.28 10 50 2400 0.1-0.5 3500 0.23 50 140 2500

The tiiickness of the tracheid cell wall is determined approximately with the assumption (for this case only ) that the tracheid is square but its lumen are round in shape and that the fraction of the cell wall in the ends of the tracheid is negligibly small:

T, = **X **

moisture content is equal to:

CW

**G^y^ is the specific gravity of the dry cell wall substance of solid wood, approximately equal **

to 1,460 kg/m^. The dry density of average Scandinavian spruce is taken as 450 kg/m^. The
* value ofA,B, D, and S],S2, S^, S4, for the representative tracheid in the three principal *
directions are calculated with die data above.

Tracheid is tapered along the radial surface at its ends for a large portion of its length. Most
bordered pit pairs are on the tapered part of radial surface. In the model, 90 percent of pits is
assumed to be on the radial surface (facing the tangential direction). The fact that most pit
"axes" (perpendicular to membrane) do not point to the three principal directions are
**accounted by choosing proper tortuosoty T2 and T3. This is especially true for longitudinal **
* diffusion, where large tortuosities have to be used. T2 and T5. are assumed to be 50 in this *
case for modeling spruce.

In the conventional drying of green wood the high tension produced as water evaporates from the cell pits forces a large proportion of the pit membrane towards the aperture until the tori cover and seal off the apertures. The aspirated tori are held on the aperture by hydrogen bonds, which prevents both vapor diffusion and liquids flow through the aspirated pits. According to Boutelje (1976) 75 percent of the pits are aspirated for the summer wood of Scandinavian spruce and 50 percent for the summer wood of pine after drying. To take account of a less value for spring wood, the attenuation factor 1 of average spruce is assumed to be 0.7 in the simulations.

In short, in the simulation of moisture transport in average spruce the data used are: Dry wood density 450 kg/m^, pit number per tracheid 50, among them 45 items are in radial face and 5 items in the tangential one. Average pit aspiration is 70%.

**3.3 Some Results of Simulations **

*This model is applicable in the entire hygroscopic range, especially from u = 2% to u = *

firstly by the curve of activation energy for bound water diffusion determined by Stamm, Skaar and Siau, figure 3, secondly by Simpson's data fitting of the Hailwood-Horrobin equation.

Some simulation results of average Scandinavian spruce are plotted in figure 6, 7, 8,9 and
*10. To meet the interests of the building industry for ö(p) and of the wood drying research *
for Dfw), they are both presented by plotting their value curves against the relative humidity
*and the moisture content respectively. The relation of 6(p) and D(w) for solid wood are *
known only obscurely before. The simulation here will also set some light on this problem.
*The simulation derived tangential, radial and longitudinal diffusivities d(p) and the *
*corresponding D(w) with 70 % pit aspiration at 23.3 °C are shown in figure 6 and figure 7. *

*d(p) in the tangential and radial directions increases pseudo-exponentially with relative *

*humidity for the most part. The curve shapes of D(w) are very different from those of S(p) *
and their values are about 10,000-100,(X)0 times smaller. In the tangential and longitudinal
*directions D(w) increases with moisture content between around u = 0 and u = 9.5, then it *
*decreases as u becomes larger. But as u increases above 20%, D(w) in tangential increases *
again. This is probably caused by the level up of the sorption isotherm near this point that
produces less dr/dC in Eq(26). The tangential and radial diffusivities are similar though not
equal while the longitudinal diffusivity is much larger.

In figure 8 are the simulation obtained diffusivities of spruce at 0 °C, 23.3 °C, 80 °C, and
*120 °C with 70% aspiration. The corresponding values ofD(w) are in figure 7 and figure 9. *
*The variation of S(p) at these temperatures is not so large, much less than that of D(w). This *
probably arises from the fact that moisture concentration in wood w is rather sensitive to
temperature and it increases much faster than the moisture concentration in the air when the
temperature increases.

The effect of pit aspiration on diffusivities is also simulated, and is presented in figure 10. It can be seen that the tangential diffusivity values at 23.3 °C distincts from each other when the percentage of pit aspiration is 0%, 70%, and 100%. The distinction is, however, very small.

8(p)(10-6 m V s )
**A: Tangential **
**B: Radial **
**C: Longitudinal **
**16 **
**8 **

### ®

**O**

_{20 40 &0 }**R e l a t i v e Humidity <"/-)**

**80**

**100**Figure 6

*Moisture diffusivity ö(p) of spruce versus relative humidity in the three principal *
directions from the present model. The temperature is 23.3 °C, pit aspiration 70%.

D(w)(10-iöm2/s)
**'10 **
**A: Tangential **
**B: Radial **
**C: Longitudinal **
**D: Tangential **
**23.3 C **
**M o i s t u r e Content (X) **
Figure 7

**6(p)(10-^ m^/s) **

**A: Tesiperature **

**20 ** **40 60 **

**R e l a t i v e Humidity (%) ** **80 ** **100 **

**Figure 8 **

**Moisture diffusivity 8(p) versus relative humidity for spruce in tangential from the ****present model. Pit aspiration 70%. **

**OCw;(lO-'öm2/s) **
**300 **
**200 **
**100 **
**A: Tenperature 120 C **
**O ** **10 20 **
**M o i s t u r e Content **
**Figure 9 **

**Moisture diffusivity D(w) versus moisture content for spruce in tangential, with 70% ****pit aspiration. **

**6(p) (10-^ m^/s) **

**8 **

**A: A l l p i t s are destroyed, f r o i present **
**B: lOX p i t are aspirated nodel ****C: 1007. p i t are aspirated **

**D: The highest values of sapttood, **
**E: The lowest values of heartwood **

**froa B e r t e l s e n s **
**experitent **
**20 40 60 **
**R e l a t i v e Humidity <%) **
**80 ** **lOO **
**Figure 10 **

**Tangential moisture diffusivity 8(p) versus relative humidity at 23.3 ^C. **

**A, B and C are values from the present model for spruce with dry density of 450 kg/m^. **
**Distributed between the curve D and E are the experimental results of Berteisen (1984) **
**for spruce with various densities from 417 to 497 kg/m^ at 23.3 °C. **

**3,4 Comparison with Bertelsen's Experiment **

**Berteisen (1984 ) measured the tangential diffusivity of spruce with the cup method at 23.3 **
**°C. He found that the moisture diffusivity differs to some extent between sapwood and **
**heartwood. His test results are replotted in figure 10 together with the simulation results **
**under the same conditions for spruce with 0%, 70% and 100% pit aspiration. The **
**diffusivities from the simulation are 3 to 5 times as large as the values from Bertelsen's **
**measurements when the relative humidity is below 50%. From around the relative humidity **
**of 70% upwards the diffusivities of the two sources almost overlap. The curve shapes and **
**variation tendencies of the diffusivities in respect to the relative humidity are very much **
**similar. **

**So the simulation results conforms well with those of Bertelsen's tests at high relative **
**humidity. And although the conformation is less satisfactory at low relative humidity, it is **
**still fairly good (note the small unit of the vertical coordinate in figure 10). **

**The deviation at low relative humidity originates probably from: (1) The tracheid structural **
**data in the simulation are of average one whereas the samples of Berteisen were prepared **
**from one specific tree. (2) The tortuosities in the simulations are to some extent chosen at **
**random since no previous data or experience is available. (3) There are inevitable inaccuracies **
**involved both in the numerical solution of the model equations and the measurement system **
**of Bertelsen's experiment, which will be discussed later. Despite these differences and **
**uncertainties, the diffusivities produced from the model are rather near to those of the **
**experiments. **

**Owing to the relatively good conformation of the simulation results to those of Bertelsen's **
**test, we may say that the simulation results presented in last section, from figure 6 to figure **
**10, may provide a useful approximation of the moisture diffusivities of average spruce under **
**the simulatied conditions. **

**3.5 Comparison with Siau's model **

**Siau ( 1 9 8 4 ) presented a model of hygroscopic moisture transport in solid wood under two **

**assumptions: **

**1. The effect of pits are negligible, only lumens and cell walls determine moisture **
**diffusivity in wood. **

**2. The different components of a cell (cell wall and lumen) that provide resistance to **
**diffusion can be ueated with analogy to the resistance of electric circuit. This means **
**that the resistances are directiy additive when they are in series and their reciprocals **
**are additive when they are in parallel. **

**Together with the concept of a volume averaged cell, these two assumptions directly result in **
**the analytical expressions of moisture diffusivities in longitudinal D L and in transverse **
**(Siau did not separate tangential and radial). Based on moisture concentration in gross wood **
**and written in the form of reciprocals for clarity, the diffusivities are: **

**(1 a)(l a') , a(l **

**-i . = (1 - a ^ ) { _ ^ J . ^ - 1 ^ ) ( 2 8 ) **

**Here a is the square root of wood porosity. and Di,i are bound water diffusivities in ****transverse and in longitudinal , and D^^ is vapor diffusivity in the air, all are based on **
**moisture concentration in the wood substances. Dy,^ is directiy from Eq(l) by converting the ****basis from moisture concentration in the air to that in the wood cell substance. In the **
**expression of longitudinal diffusivities a ratio of 1/100 for cell widtii and lengtii is supposed. **
**If the resistance of wood cell walls is neglected when it is in parallel with lumens, the **
**diffusivity expressions above are simplified to: **

**1 D. p **

**D**

** ^—**

**^—**

### nO)

**^ l - a ^ I ^ b t ^ O O U l - a ) D _{vs }**

**Siau's model is pretty in form, relatively simple and easy to use. It has been believed to be **
**able to produce reasonable estimations for the magnitude order of wood diffusivities. The **
**drawback of this model is that it is not sufficiently sophisticated. For wood of any property, **
**for wood having all pits aspirated or destroyed, it always predicts identical diffusivity when **
**their densities are identical. Siau directly applied Eq(l) as the effective water vapor **
**diffusivity without dividing it by a factor which certainly made his model **
**invalid when the temperature is higher than 50 °C. But without realising this, Siau (1984, **
**P. 164) used his model to temperature as high as 100 °C. Finally the analogy of moisture **
**diffusion in wood to the electric circuit seems to be not strictly sound since it is not a linear **
**system. The resistances to moisture diffusion are concentration dependent, they are not **
**simply additive. **

**The present model does not bear these disadvantages. It has incorporated in itself nearly all **
**the factors that are possibly influential to isothermal moisture diffusion in conifer wood, and **
**expressed them on the basis of physical understanding in such a flexible way as to be **
**adaptable to the cellular structures of distinct conifer woods. So it can be used to a wood **
**species by taking detailed considerations to its cellular structural features. It is also suitable **
**for woods that has undergone various artificial treatments or natural processes that have **
**alterred the cell structure to some degree. For example, simulations can be made for a wood **
**plank that has been impregnated with some chemicals so that parts of its lumens and pores **
**are blocked, or for a wood block whose pits are all destroyed by alkalis, enzymes or by **
**water storage. But on the other hand, the present model is more time-consuming to use, and **
**some trial and error work is needed to convert the structural features of a kind of wood to the **
**various sizes of the representative tracheid if good predictions of diffusivities are anticipated. **

**In figure 11 the transverse and longitudinal diffusivities Dfwj of solid wood with dry density **
**of 500 kg/m3 at 20 °C and 80 presented by Siau (1984) from his model are reproduced. **
**Plotted together are also the diffusivity curves from the present model for average **
**Scandinavian spruce at 23.3 °C and 80 °C with all pit aspirated. Siau showed straight lines **
**for the transverse diffusivities on the graph with logarithmic vertical coordinate, which is **
**apparently not derived from Eq(27) or (29), but from a further simplification of Eq(29) that **
**he originally stated to be vaHd only when moisture content is below 15%: **

**From figure 11 it can be seen that the diffusivity curves predicted from the present model for **
**spruce are nearly in similar ranges and has similar variation tendencies to those from Siau's **
**model. The higher diffusivities predicted by the present model is presumably caused mainly **
**by the smaller dry wood density than that in Siau's model. The density is expected to affect **
**wood diffusivity a great deal because it determine the sizes of lumens and the moisture **
**diffusion in lumens is by far faster than in wood call wall. The much larger curvatures of the **
**diffusivity curves from the present model may be attributed partially to the curve fitting of the **
**activation energy with quadratic equations in Eq(lO), where Siau adopted the linear **
**approximation. **

**Therefore, although very different approaches are taken in the present model and in Siau's **
**model, and although the wood simulated by the two models have some differences, the **
**predicted diffusivities showed similarities and are in similar range. **

**10 15 20 **

**Moisture Content (%) **

**25 **

**30 **

**Figure 11 **

**Moisture diffusivities D(w) versus moisture content predicted by Siau's model ****(dotted curves) and present model (continuous curves). **

**Siau's model: A, B — Tangential, temperature 20 °C and 80 ****C, D — longitudinal, ; 20 and 80 »C **

**dry density 500 kg/mS, pits are neglected **
**Present model: E , F — Tangential, temperature 23.3 ^'C and 80 **

**GJH — longitudinal, ; 23.3 »C and 80 »C **
**dry density 450 kg/m3,100% pit aspiration **

**4. ANALYSES O F M O I S T U R E TRANSFER T H R O U G H **

**MOVING AND S T I L L AIR **

**When the cup method and the sorption method are employed to the measure moisture **
**diffusivity, the resistance to moistiu-e transport by the boundary layer between the moving **
**bulk air and the sample surface is usually neglected (Liu Tong, 1986). This may cause some **
**error in the measured results. The problem has scarcely been investigated and some analyses **
**will therefore be made here with boundary layer theory. For the cup method, the stagnant air **
**layer inside the cup can also hinder moisture movement through it. This commonly ignored **
**problem is to be studied with the equation of binary gas diffusion. Analyses in these two **
**problems here would hopefully be able to cast some light on them and lead to a better **
**understanding and utilization of the two important measurement techniques. **

**4.1 Moisture Transfer under Forced Convection **

**Consider a piece of wood whose surface moisture content is or Wy Air that has a moisture ****concentration poo is blown parallelly to the lumber with velocity U. Due to the shear stresses ****between the air and the surface, the air next to the surface is brought to rest when it reaches **
**the leading edge of the lumber. The shear stresses in the air subsequently retard the flow of **
**the air in a very small thickness known as boundary layer, figure 12. **

**Figure 12 **

**Boundary layer and **

**the velocity **

**distri-bution of the flow **

**air over a piece of **

**wood **

**The laminar boundary layer continues to thicken along tiie surface. If the lumber is **
**sufficientiy long a point known as the critical lengtii would be reached after which the air **

**flow of the boundary layer becomes unstable and turbulent. **

**The boundary layer opposes moisture transfer through it and bring about surface resistance. **
**The mass transfer between the bulk air and the wood surface through the boundary layer can **
**be described by: **

**Hv = Pav(Ps - P oo) ** **(31) **

**where is the average mass transfer coefficient **

**From the boundary layer theory (Hines and Maddox, 1985) it is known that when a **
**Sherwood number Sh = p^v^/Sf^ is above 25 (which is in general fulfilled for air and water ****vapor system as d^^ is very small), the mass transfer resistance through the boundary layer is ****predominant for forced convective mass transfer. Under such conditions, the average mass **
**transfer coefficient for the fluid flow across a flat plate is: **

**5 i 1 **
**0.664 i ^)(Sc)^ ( R e ) ^ ****Re < 500,000 **
**(laminar flow) **
**p^= -iil<0.0365Re - 853) **
**4 **
**0.0365 x ^ x R e ^ **

**(32) (partial laminar and **
**partial turbulent flow) **

**500,000 < Re < 10 **
**(turbulent flow) **

**where v is Uie kinematic viscosity of the air, L the length of the wood lumber in the air flow ****direction. 5c and Re are Sherwood number and Reynolds number, expressed in this case ****as: **

**b e - g **
**m **

**Re = U L **

**v can be obtained rather accurately with: **
**v = (12.5 + 0.11 T.) X 10-6 (in2/s) **

**Here T^. is the temperature in Celsius. The average mass transfer coefficient is dependent on ****air velocity, length of the wood lumber and temperature. It is not influenced by the flux of **
**moisture through the boundary layer and inside the wood. So the analyses in this chapter is **
**valid for both steady- state (cup method) and transient (sorption method) moisture transport. **

**First, check whether the boundary layer in ordinary sorption and cup methods is laminar or **
**turbulent. From the expression of Reynolds number the critical length is: **

**L c , = 5 X 10+5 vAJ = ( 6 . 2 5 + 0.055Tc)AJ **

**at Tc = 20C, U = 3m/s,**** \.^ = 2A5**** m **

**U = 5m/s, Lcr= 1.47 m **
**U = 8m/s, Lcr = 0.919m **

**Therefore it can be concluded that with the cup and sorption methods the boundary layer is **
**always laminar because the sample lengths never exceed 0.9 m. **

**Assume that the length of the wood lumber is 0.1m, the average mass transfer coefficient is **
**calculated with respect to air velocity at the temperatures of 5 °C, 23.3 °C and 80 °C **
**respectively, figure 13. It can be seen from figure 13 that the average mass transfer **
**coefficient increases proportionally with the square root of the air velocity. Temperature has a **
**relatively weak influence on the average mass transfer coefficient **

**In figure 14 the mass transfer coefficient with respect to air velocity for three situations are **
**plotted: (1) Wood lumber length L=lm, temperature Tc=80 »C, (2) L=5m, Tc =80 and (3) **
**L=5m, Tc =130 °C. In the regime of laminar flow, the average mass transfer coefficients are **
**less for the two longer lumbers. But when turbulence appears around the air velocity of 2.5 **

**m/s they increase rapidly, surpassing that of the 1 m long lumber when the air velocity is **
**above 4 m/s. So the occurrence of turbulence on wood lumber of large length will effectively **
**reduce the surface resistance. **

**The difference of relative humidity between the lumber surface and the bulk air is **
**proportional to the moisture flux through it. When the average mass transfer coefficient is **
**known, it can be calculated, from Eq(31), Eq(16) and Eq(17): **

**From figure 13 and figure 14 it is clear that the velocity should be no less than 1 m/s in **
**order to keep this relative humidity difference small. In the test with the sorption method the **
**flux decreases rather rapidly from the initial large value and so the value of f^^ - (poo) would ****also change in such a way. Consequently, for the sorption method the moisture transfer is **
**most sensitive to surface resistance in the initial sorption stage. In this stage a high air **
**velocity is imperative. In the cup method, the flux of interest is constant, so the **
**coiresponding relative humidity difference is also a constant. Proper air velocity (larger than **
**1 m/s ) should be kept to make this difference small. By the way, if a sample has a very **
**large diffusivity and a constant flux , much larger than those of wood samples, the air **
**velocity should also be much larger. The difference of relative humidity and consequentiy the **
**proper value of air velocity depends primarily on the magnitude of the flux. **

**Kav ( l O . E - 2 m/s) **

**A i r V e l o c i t y (m/s) **

**Figure 13 **

**Average mass transfer coefficient versus air velocity for a sample of 10 cm **
**along the air flow direction. Temperatures are 5 °C, 23.3 °C and 80 °C. **

**Kav ( l O . E - 3 m / B ) **

**A i r V e l o c i t y <m/s) **

**Figure 14 **

**Average mass transfer coefficient versus air velocity. **
**Curve A: Sample length Im, temperature 80 °C **
**Curve B: Sample length 5m, temperature 80 °C **

**(the dotted branch would be assumed if **
**turbulence did not occur). **

**4.2 Moisture Transfer Through Still Air **

**When cup metiiod is used to measure moisture diffusivity, the stagnant air layer inside the **
**cup between the sample and the salt solution or drying agent has some resistance for moisture **
**transport figure 15. **

**Figure 15 **

**Wood sample and **

**cup in the cup method. **

**A : Sample **

**B : Cup **

**C : Salt solution or **

**drying agent **

**The equation of water vapor diffusion in still air in the differential form is expressed in **
**Eq(3). Integration of the molar flux along the height of the stagnant air layer results: **

**N = • **

**Here Xj and Xj, are the molar water vapor concentration in the air on the wood surface and at **
**the bottom of the stagnant air layer. The corresponding mass flux expressed with mass **
**concentration p^^ is: **

**p M 6 p M - p **
**n = l L _ ^ x ln(12_JL_-lL **

*** h ** _{p M - p. }) **(34) **

**p - p. p M**

** 5 **

**Where (p) = , P,, = .**

*** p M - p "^^^^log**

**l n ( l S - J ^ )**

**p M - p.**

**w '^b**

**When Ply and the flux Uy are known (p^ is determined by the salt solution or drying agent ****used, the flux is measured in experiment), can be calculated with: **

**n **

**V **

**Pc = — + P **

**Pst ** **'b (36) **

**The unknown is contained in the expression of pg^^ In the calculation an initial estimated ****Pg can be substituted into Eq(36) and better values are derived with successive ****approximation until satisfactory value is obtained. The difference of relative humidity in the **
**air between the wood surface and at the bottom of the stagnant air layer can then be directly **
**calculated with pg and p^,: **

**<t>s-<l>b = <t)tX(Ps-Pb) (37) **

**Here some calculations with conditions quite probable in the cup method are made. Assume **
**that at temperature 20 °C, the height of the stagnant air layer is 1 cm, 2 cm and 3 cm **

**respectively. The relations of relative humidity difference (0^**

** -**

**(f>i,)****and hte moisture flux**

**calculated with the above equations are illustrated in figure 16. It can be seen that ((p^ - <}>b) ****increases almost linearly with the flux. When flux is 1.4 x 10'^ kg/m^s, ((p^ - (pi,) is about ****3.3%, 6.5% and 9.8% respectively - rather large indeed. The slope of the line increases **
**proportionally with the height of the stagnant air layer. The slight curvature of the Uiree lines **
**is caused by the factor fZ-Xyj in Eq(3). **

To investigate the effect of temperature, calculations are made for the temperatures of 5 °C,
20 °C, and 35 °C, taking the height of the stagnant air to be 2 cm, figure 17. As the
temperature increases the resistance of the still air decreases apparently. This should be
attributed to the temperature dependence of vapor diffusivity in bulk air 5^ and the saturation
**vapor pressure contained in (p^. Both quantities increases with temperature. **

Calculations are also made for the temperature 20 °C and chamber height 2 cm with relative
humidities at the bottom of the air space being 66%, 33% and 0%, figure 18. This is for
investigating whether the level of the lower relative humidity has some influence on** ((ps-^Pb) • **

The answer is negative. The three curves nearly overlap completely.

Berteisen (1984) made experiment with drying agent in the cup* ((pi,=0)* at temperature 23.3

^C. One group of his spruce heartwood samples have the thickness of 8.8 mm. When the
relative humidity outside the cup is 92.1%, 52.4% and 34.4% the measured average moisture
**flux 2.57 X 10-6, 0.253 x lO'^ and 0.0969 x 10-^ kg/m2s respectively. Berteisen did not **
state how large the distance between the drying agent and the wood surface was. Using his
temperature and flux data, we now calculate the relative humidity difference between the
drying agent and the sample surface in relation to the distance between them. The results are
plotted in figure 19. We can see that for the two large fluxes the resistance of the air space in
the cup brought about relatively large difference. As the air space is 1.5 cm high, which is
most probable in a cup test, the difference of relative humidity is about 7.2%, 3.4% and
0.36% for the three fluxes.

We further consider for Bertelsen's test the surface resistance outside the cups. Berteisen measured the air velocities to be 3, 3.1 and 3.3 m/s. We take the average as 3.1 m/s. From figure 13 it can be read that at temperature 23.3 °C and air velocity 3.1 m/s the average mass transfer coefficient is about 6.45 x lO^^ m/s if the samples are assumed to be 10 cm long in air flow direction. Had the air velocity been 0.5 m/s, the average mass transfer coefficient would be around 3.0 x lO^^ m/s. With these two values the difference of relative humidity between the bulk air and the wood surfaces outside the cups are calculated and listed below, together with the data for the cases inside the cups:

Difference of Relative Humidity of Cup Test

produced from Bertelsen's data (1984) with two reasonable assumptions (1) the height of the air space inside the cup is 1.5 cm.

(2) samples are 10 cm long in air flow direction) Outside the cup(%)

(between the bulk air and wood surface) Flux air velocity (10-6

kg/m2s) 3 m/s 0.5 m/s 2.57 0.19 0.41

0.253 0.019 0.040 0.0969 0.0072 0.016

Inside the cup (between drying agent

and wood surface)

7.2 3.4 0.36

The deviations of the relative humidities on sample surface from the expected values is much
larger inside the cup than outside it. It may be concluded consequentiy that the stagnant air
space inside the cup exerts a much larger resistance to moisture diffusion than the boundary
layer on the outside sample surface. This is tme even when the velocity of the air flow is
rather low.
**>• ****100 200 **
**Moisture Flux (10-8 kg/m2«s) **
**300 **
Figure 16

Difference of relative humidity versus moisture flux through the stagnant air layers that are 1, 2, and 3 cm high respectively. Temperature is 20 ^C. The lower relative humidity is zero.

**10 **
**^ 8 **

**•e-flC**

**• 4**

**of **

**of**

**p/ **

o **p/**

**100 200**

**M o i s t u r e F l u x (10-8 kg/m2ts>**

**300**

**Figure 17**

**Difference of relative humidity versus moisture flux through a 2 cm thick stagnant **
**air space at temperatures of 5*C, 20 °C and 35 ^C. The lower relative humidity is **
**zero. **

**l o **
8
**E **
**2**** A **
**a> **
**4 **
**09 **
**O **
**C **
**O) **
**i **
**-O)** o
**C) **
**Hb=667.-Hb=33y. **
**Hb=oy. **
**100 200 **
**M o i s t u r e F l u x (10-8 kg/fn2»s) **
**280 **
**Figure 18 **

**Difference of relative humidity versus moisture flux through a 2 cm thick stagnant **
**air space at 20 °C. The lower relative humidity are 1 %, 33% and 66%. **

**=0.0969E-6 kg/m2*s **
**F l u x **

**( > ** **10 20 30 40 **

**Height o f S t i l l A i r Space (mm) **

**Figure 19 **

**Difference of relative humidity versus the height of the air space inside the cup at **
**three flux values that Bertelsen(1984) obtained in his test for spmce samples. **